Macromolecules 1992,25, 5559-5560
Characterization of Interchain Interactions in Perdeuterated Bisphenol-A Polycarbonate by Residual-Proton Solid-state NMR 7
Patricia Lani Lee and Jacob Schaefer' Department of Chemistry, Washington University, St. Louis, Missouri 63130 Received May 12,1992 Revised Manuscript Received July 14, 1992
i I t has been postulated that interchain cooperativity of molecular motion is responsible for many of the useful engineering properties of bisphenol-A polycarbonate.' Previous experiments using solid-state NMR to probe this phenomenon have focused on interpreting the spectra of either a single d e ~ t e r i u m or~a~directly ~ bonded carbonproton pair on one chain.4 In both instances, direct observation of dynamics is limited to a single chain; the effect of other chains on the properties of the detected nucleus must be inferred. Study of the dipolar interaction of two nuclei, each on a separate polymer chain, leads more directly to information about the cooperative motions of interest. Detection of a proton-proton pair is preferable to that of a carbon-carbon pair due to the proximity of interchain protons and the excellent sensitivity arising from the large proton gyromagnetic ratio. However, the broad featureless NMR signal from protons at natural abundance is generally difficult to interpret. This problem can be circumvented by the use of perdeuterated compounds containing only residual protons. The residual-proton NMR spectra of perdeuterated bisphenol-A polycarbonate (PCdl4) and the bisphenol-A monomer (BPA-dls) shown in Figure 1were obtained at 60MHz with 1852-Hzmagic-anglespinning. A 90-~-180-~ pulse sequence was used with T equal to an integral number of rotor periods. The average level of residual protonation was quantified by solution-state NMR and found to be about 1% for both PC-dr4 and BPA-dl6. In both samples the methyl groups were preferentially labeled. The ratio of aromatic signal to methyl signal was found to be 2:l instead of the expected 43. At low concentration, protons behave as a rare spin-'/n with the NMR spectrum dominated by heterogeneous rather than homogeneous interactions. Even at relatively low spinning frequencies, complete separation of sidebands is achieved, indicating that proton spin-pin communication is limited. Aromatic and methyl-proton resonances are almost resolved at 60 MHz, although the high-field peak of P C 4 4 has an important contribution from water which is better resolved at 300 MHz (Figure 2, left). This water is exchangeable with DzO and can be removed by heating the sample under vacuum. Upon exposure to the atmosphere the water is reabsorbed almost immediately. The resonance position of the water at higher field than that of the methyl protons is consistent with isolated water in an organic matrix.586 The size of the residual water sidebands (Figure 2, top left) and their insensitivity to deuterium decoupling (spectrum not shown) indicate that the water is tumbling almost isotropically. Therefore, its predominant NMR interaction is intramolecular proton-proton dipolar coupling. The persistence of pronounced 60-MHz aromatic and methyl-proton sidebands with 1852-Hz spinning (Figure 1, top; Figure 2, right) requires an interaction strength greater than 2 kHz. This is much larger than either the averageTe8idudpTOton-pTOton dipolar coupling (cf. below)
rotor periods, v
-2 -3 kHr
Figure 1. Residual-protonNMR spectra at 60 MHz with 1852Hz spinning of polycarbonate-dlc (top) and bisphenol-A-dle (bottom) obtained using a 90-T-180-7 pulse sequence with T equalto an integralnumber of rotor periods. The broad sidebands for T = 1rotor period for bisphenol-A-dls are due to clusters of exchangeable OH protons. The ppm scale is referenced to the aromatic-proton peak. 3125 - Hz Spinning 300 MHr
1852-Hr Spinning 60 MHr
1 " " I " " I " " I
Figure 2. Proton NMR intensitiesof centerbande(bottom)and upper first spinningsidebands (top)for polycarbonate-d1, at 300 MHz (left) and 60 MHz (right). The relative contribution from
water is lese in the sidebands than the centerband. The ppm scale is referenced to the aromatic-proton peak.
or the proton chemical shift anisotropy at low field. We attribute the kHz-range interaction in PC-dl4 to protondeuterium dipolar coupling. This is supported by the reduction of sideband intensity with on-resonance deuterium decoupling at 30 kHz (spectrum not shown). By contrast, the residual proton spectrum of perdeuterated bisphenol-A (BPA-dls), the monomer precursor of PCd14, has no detectable spinning sidebands (Figure 1, bottom). Because intramolecular proton-deuteron distances are similar for both BPA and PC, the interactions giving rise to the proton sidebands in PC-dl4 must be interchain. This result leads to the unexpected conclusion that, for the phenyl rings and isopropylidene groups, the average packing in the glassy polymer is more dense than in the crystalline monomer. The decay in intensity seen for PC-dId as T increases (Figure 1,top) defines the natural TZof the sample, which arises from the combined effect of molecular motion and
0024-9297/92/2225-5559$03.00/00 1992 American Chemical Society
Macromolecules, Vol. 25, No. 20,1992
5560 Communications to the Editor DRAMAIT? RATIO AT 300 MHz
u A n h " * A A A ' F A
Figure 3. Ratio of DRAMA to Tz signal intensities for the residual aromatic protons of polycarbonate-dlrand bisphenolA-dle. The intensities for the latter are influenced over the first rotor periods by contributions from the exchangeable protons (see Figure 1, bottom). All data were obtained at 300 MHz with 3125-Hzmagic-angle spinning. DRAMA dephasing was achieved by 5-ps sI2 pulses placed at lIqTrand 3/4Tr.
deuterium-proton dipolar coupling. If, in addition to the refocusing K pulse, two d2-proton pulses are applied during each rotor cycle, further dephasing occurs due to reintroduction of the proton-proton dipolar interaction of isolated proton pairs that had been suppressed bymagicangle spinning. This effect has been described by Tycko and Dabbagh, and the pulse sequence has been given the name "DRAMA" for dipolar recovery a t the magic angle.7 The ratio of the DRAMA signal intensity to the Tz signal intensity removes the natural decay, leaving only the dephasing caused by proton-proton dipolar interactions. For BPA-dls, the 7r/2 pulses have virtually no effect and the ratio is approximately one (Figure 3), which means that there are no significant proton-proton dipolar couplings. For Pcd14, however,the denser packing introduces interchain proton-proton interactions which cause the additional decay seen in the DRAMA/Tz ratio (Figure 3).
The DRAMA dephasing corresponds to an average protonproton dipolar coupling of 350 HzS7More than half of the protons are affected because of large-amplitude molecular motions in the polymer, not present in the crystalline BPA monomer, which allow each proton to come into contact with many different sites, thereby increasing the chance of a proton-proton dipolar coupling. At lower temperatures some of these motions are frozen out, reducing the number of protons which have H-H interactions. This causes the DRAMA/Tz ratio to shift to higher values (Figure 3). The shift is limited because even a t -100 "C most of the phenyl rings are still undergoing 180° flips at a rate that is fast compared to the 350-Hzproton-proton ~oupling.~>~ The conclusion that polycarbonate has shorter intermolecular distances than its crystalline monomer is based on both the DRAMA results and the comparison of BPAdI6and PC-dId spinning sidebands. Analysis of the results of heteronuclear NMR experiments on selectively labeled polycarbonates and computer simulations of protonproton and proton-deuterium interactions are currently underway to extract accurate internuclear distances between polycarbonate chains in the glassy state. Results will be submitted to this Journal.
Acknowledgment. This work has been supported by NSF Grant DMR9015864. References and Notes (1) Nielaen, L.E.Mechanical Properties of Polymers; Reinhold Publishing Corp.: New York, 1962;p 125. (2) Spiess, H. W.Colloid Polym. Sci. 1983,261,193. (3) B l h i c h , B.; Spiess,H. W. Angew. Chem.,Znt. Ed. Engl. 1988, 27, 1655. (4) Schaefer, J.; Stejskal, E. 0.; McKay, R. A.; Dixon, W. T. Macromolecules 1984,17,1479. (5) Fyfe, C.; Randall, L.;Burlinson, N. Chem. Mater. 1992,4,267. (6) Derome, A. E. Modern NMR Techniques of Chemistry Research; Pergamon Press: Oxford, 1987;p 34. (7) Tycko, R.; Dabbagh, G. Chem. Phys. Lett. 1990,173,461.